Journal of Nanomaterials

Volume 2008 (2008), Article ID 682920, 4 pages

http://dx.doi.org/10.1155/2008/682920

## Field Emission from Self-Assembled Arrays of Lanthanum Monosulfide Nanoprotrusions

^{1}Equipe Emission Electronique, LPMCN-CNRS, Universite Claude Bernard Lyon 1, 69622 Villeurbanne, France^{2}Department of Electrical and Computer Engineering and Computer Science, University of Cincinnati, Cincinnati, OH 45221, USA^{3}Materials and Manufacturing Directorate, Air Force Research Laboratory, Wright-Patterson AFB, OH 45433, USA^{4}Institute for Microstructural Sciences, National Research Council, Ottawa, ON, Canada K1A OR6^{5}Department of Electrical and Computer Engineering, Virginia Commonwealth University, Richmond, VA 23284, USA

Received 30 October 2007; Accepted 10 January 2008

Academic Editor: Donglu Shi

Copyright © 2008 V. Semet et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The field emission properties of LaS nanoprotrusions called nanodomes, formed by pulsed laser deposition on porous anodic alumina films, have been analyzed with scanning anode field emission microscopy. The voltage necessary to produce a given field emission current is 3.5 times less for nanodomes than for thin films. Assuming the same work function for LaS thin films and nanoprotrusions, that is, 1 eV, a field enhancement factor of 5.8 is extracted for the nanodome emitters from Fowler-Nordheim plots of the field emission data. This correlates well with the aspect ratio of the tallest nanodomes observed in atomic force micrograph measurements.

The promise of producing extremely high current densities in near-vacuum with no external source (such as heater, primary electron-beam, or intense light source) has generated significant interest in robust, reproducible, and field-emission-based cold cathodes [1, 2]. Several promising approaches to achieving cold cathode emission from a dense array of nanoscale field emitters have been investigated including metallic field emitter arrays (FEAs) or Spindt emitters [3], carbon nanotube (CNT) arrays [4], and arrays of semiconductor nanowires [5–9]. To date, metallic FEAs with uniformly high emission have been difficult to fabricate. They are prone to failure and present long-term reliability problems [3]. Carbon nanotubes (CNTs), on the other hand, can be fabricated easily, but the emission current density that they can support, while adequate for some applications, is currently not enough for mainstream high power devices such as traveling wave tubes (TWTs). Semiconductor and semimetallic nanowires therefore appear as perhaps the most promising route to realizing field emitters that can support a large total emission current, in particular if regular high density arrays of them can be fabricated in a self-assembled growth mode. Moreover, to achieve high current densities under low applied voltage, the field emitter material must have low work function. Rare earth monosulfides are therefore ideal for this purpose.

Recently, we reported the first successful deposition of lanthanum monosulfide (LaS) thin films on Si substrates using pulsed laser deposition (PLD) [10, 11]. They were flat layers composed of nanocrystallites having dimensions of the order of 5 nm. The scanning anode field emission microscopy (SAFEM) technique was used to measure the field emission (FE) properties of these LaS thin films (about 0.1 m thick) [12]. It was shown experimentally that electrons are easily extracted by FE from patchwork areas of few nanometer dimensions having a measured effective work function of 1 eV, corresponding to some outcropping LaS nanocrystallites with (100) orientation, embedded in a2.8 eV work function surface related to other crystallographic orientations. A LaS thin film obtained by PLD can therefore be an excellent field emitter material, especially if we can take advantage of a field enhancement factor at the tip of nanoscale protrusions formed from such material.

In this letter, we report FE properties of arrays of LaS
nanoprotrusions self-assembled with a density as high as 10^{9}/cm^{2}.
These nanoprotrusions, called nanodomes and nanodots hereafter, are produced
when LaS is pulse-laser-deposited on nanoporous anodic alumina films containing
hexagonal arrays of cylindrical pores that are 50 nm wide and 500 nm deep.
The details of the self-assembly growth of arrays of nanoprotrusions using a
porous anodic alumina film as a template are given in [13].

The nanodomes are cone-shaped LaS structures with base
diameter ranging from 50 to 100 nm and height ranging from 100 to 150 nm.
They were found to grow on the boundaries separating regions of the anodic
alumina film that have near perfect pore ordering. Their density is 10^{9}/cm^{2},
as extracted from the field emission-scanning electron micrographs (FE-SEM) and
atomic force micrographs (AFM) such as those shown in Figures 1 and 2,
respectively. In addition to nanodomes, nanodots (or quantum dots) of LaS
nucleate on top of the alumina islands between adjacent pores. These are sites
of minimal strain. The dots have a diameter 50 nm, a density equal to the
pore density (10^{10}/cm^{2}), and an aspect ratio less
than 1.

The SAFEM technique was used to measure the FE
current-voltage (*I*-*V*) characteristics at different surface locations. As the
nanowires are buried inside the pores, they contribute very little, if any at
all, to the net FE current. Moreover, FE measurements from the arrays of
nanodomes and nanodots were possible because the regions joining adjacent
nanodomes and nanodots are covered with a thin percolating network of LaS over
the entire array. Its presence was confirmed by measuring a low resistance
value of about 2 Ohms between two electrical contacts about 1 cm apart. For
each location, a full set of *I*-*V* characteristics (total measured current versus
applied voltage) for different values of *d*,
the distance between the cathode surface and the probe ball, was measured. This
set of measurements was then analyzed in order to extract the apparent current
density *α **J* versus actual
applied local field *γ **F*, where *γ* is the local geometrical field enhancement at
the surface of the cathode [14], *F* is the notional electric field at
the corresponding flat LaS cathode surface (when *γ*= 1), a factor taking into account the actual
emitting area, and *J* the notional FE current density. In Figure 2, we see that
the nanodome structures dominate the landscape and therefore they have the
highest field enhancement factor *γ*. The relative contribution of the nanodots to the total FE current
is minor due to a smaller value of the associated with them. In all probability, the majority of
the measured FE current is then extracted from the highest nanodomes.

*I*-

*V*data to the surface morphology of the cathodes, both SAFEM measurements were performed with the same probe ball-to-cathode distance m. Typical

*I*-

*V*characteristics are shown in Figure 3 for both thin film and nanodome cathodes. We found that in order to extract the same total FE current, the applied voltage for nanodome cathodes was 3.5 times less than that for thin film cathodes. This indicates clearly the contribution of the protruding geometry of the nanodomes to the FE current.(2)The total FE current versus applied voltage (

*I*-

*V*) characteristics were measured for different values of the probe-ball-to-cathode-surface distance

*d*. From these data, the apparent current densities ( and ) as a a function of the applied local field were extracted [15, 16], assuming that the applied local electric field included the local enhancement factor

*γ*, that is, and , for LaS thin film and nanodome cathodes, respectively.

*α*

_{tf}and

*α*

_{nd}are parameters taking into account the actual emitting areas from low work function nanocrystallite zones [12] and the density of emitting nanodomes. The corresponding Fowler-Nordheim plots (ln(

*α*

*J*/(

*γ*

*F*)

^{2}) versus 1/

*γ*

*F*) of the data are shown in Figure 4. As a result of the field enhancement factor, the emission area for nanodome cathodes was restricted to the nanodome apexes. The actual current densities

*J*extracted from each nanodome are then much more important than the values of the apparent current densities in the plot of Figure 4. The exact estimation of the ratio

*α*

_{nd}/

*α*

_{tf}would require a self-consistent approach, which is in progress, but one can estimate it in first approximation to be proportional to the inverse of the density of the emitting nanodomes. This ratio could be in the range of 10

^{4}to 10

^{5}.(3)The FE analysis for both cathodes, presented in the previous paragraph, was limited only to the region where the analytical FE relation developed by Murphy and Good is applicable [15, 16]. Under such conditions, the slopes

*m*and

_{tf}*m*of the Fowler-Nordheim plots are, respectively, proportional to

_{nd}*Φ*

^{3/2}/

*γ*

_{tf}and

*Φ*

^{3/2}/

*γ*

_{nd}, where

*Φ*is the effective work function of the cathodes. In Figure 4, a straight line fit to the Fowler-Nordheim plots of the data gave slope values

*m*= −0.4155 and

_{tf}*m*= −0.0716 for LaS/Si and nanodome cathodes, respectively.(4)Under the assumption that the nanodome cathodes have the same effective work function as the planar cathodes on Si, that is,

_{nd}*Φ*1eV, [12] the ratio of the slopes extracted from the Fowler-Nordheim plots is equal to the inverse ratio of the field enhancement factors. Since AFM measurements of LaS thin films on Si substrates have shown that surface corrugation is negligible [10, 11], the error introduced by taking

*γ*

_{tf}= 1 is minor. Under this assumption,

*γ*

_{nd}= 5.8. This value is in very good agreement with the geometrical aspect ratio of the tallest nanodomes observed by AFM [13].

In conclusion, the SAFEM technique was used to demonstrate
successful FE from LaS nanodomes grown by PLD on top of flexible alumina
templates. The SAFEM measurements were found to be reproducible after a
period of several months without taking any special precaution to store the
template. LaS nanodome arrays are therefore very stable field emitters with a
work function around 1 eV. Even though not discussed
here, cross sectional FE-SEM images have shown that LaS nanowires grow inside
the pores with a density of 10^{10}/cm^{2}. The nanowires have
a diameter of 50 nm and a maximum length equal to the length of the pores (500 nm) [13]. This
density could approach 10^{11}/cm^{2} by using templates with
pores size down to 10 nm. Actually, the exposure of the tips of the LaS
nanowires filling the pores can be done by etching the back aluminum substrate
and the small alumina barrier at the bottom of the pores, which could lead to
field enhancement factors for the LaS nanowires more comparable to those
reported for CNTs. This would lead to a much lower threshold voltage for field
emission compared to the one reported here and a
large increase in the density of nanoemitters culminating in the realization, therefore the realization of flexible cold cathodes using a self-assembling process with reliable and low cost production.

#### Acknowledgment

The work at the University of Cincinnati and Virginia Commonwealth University is financially supported by the US National Science Foundation under the collaborative GOALI Grant ECS-0523966. Part of this work was performed by M. Cahay under the Air Force Summer Fellowship Program, Contract No. FA9550-07-C-0052.

#### References

- A. G. Rinzler, J. H. Hafner, P. Nikolaev et al., “Unraveling nanotubes: field emission from an atomic wire,”
*Science*, vol. 269, no. 5230, 1550 pages, 1995. View at Publisher · View at Google Scholar - R. H. Baughman, A. A. Zakhidov, and W. A. de Heer, “Carbon nanotubes—the route toward applications,”
*Science*, vol. 297, no. 5582, 787 pages, 2002. View at Publisher · View at Google Scholar - D. Temple, “Recent progress in field emitter array development for high performance applications,”
*Materials Science and Engineering R*, vol. 24, no. 5, 185 pages, 1999. View at Publisher · View at Google Scholar - M. Mauger, V. T. Binh, A. Levesque, and D. Guillot, “Freestanding vertically aligned arrays of individual carbon nanotubes on metallic substrates for field emission cathodes,”
*Applied Physics Letters*, vol. 85, no. 2, 305 pages, 2004. View at Publisher · View at Google Scholar - Y. B. Li, Y. Bando, D. Golberg, and K. Kurashima, “Field emission from ${\text{MoO}}_{3}$ nanobelts,”
*Applied Physics Letters*, vol. 81, no. 26, 5048 pages, 2002. View at Publisher · View at Google Scholar - Y.-H. Lee, C.-H. Choi, Y.-T. Jang et al., “Tungsten nanowires and their field electron emission properties,”
*Applied Physics Letters*, vol. 81, no. 4, 745 pages, 2002. View at Publisher · View at Google Scholar - J. Chen, S. Z. Deng, N. S. Xu et al., “Field emission from crystalline copper sulphide nanowire arrays,”
*Applied Physics Letters*, vol. 80, no. 19, 3620 pages, 2002. View at Publisher · View at Google Scholar - C. Y. Zhi, X. D. Bai, and E. G. Wang, “Synthesis and field-electron-emission behavior of aligned GaAs nanowires,”
*Applied Physics Letters*, vol. 86, no. 21, Article ID 213108, 3 pages, 2005. View at Publisher · View at Google Scholar - R. C. Wang, C. P. Liu, J. L. Huang, S.-J. Chen, Y.-K. Tseng, and S.-C. Kung, “ZnO nanopencils: efficient field emitters,”
*Applied Physics Letters*, vol. 87, no. 1, Article ID 013110, 3 pages, 2005. View at Publisher · View at Google Scholar - S. Fairchild, J. Jones, M. Cahay et al., “Pulsed laser deposition of lanthanum monosulfide thin films on silicon substrates,”
*Journal of Vacuum Science & Technology B*, vol. 23, no. 1, 318 pages, 2005. View at Publisher · View at Google Scholar - M. Cahay, K. Garre, X. Wu, D. Poitras, D. J. Lockwood, and S. Fairchild, “Physical properties of lanthanum monosulfide thin films grown on (100) silicon substrates,”
*Journal of Applied Physics*, vol. 99, no. 12, Article ID 123502, 6 pages, 2006. View at Publisher · View at Google Scholar - V. Semet, M. Cahay, V. T. Binh, S. Fairchild, X. Wu, and D. J. Lockwood, “Patchwork field emission properties of lanthanum monosulfide thin films,”
*Journal of Vacuum Science & Technology B*, vol. 24, no. 5, 2412 pages, 2006. View at Publisher · View at Google Scholar - M. Cahay, K. Garre, J. W. Fraser et al., unpublished.
- R. G. Forbes, C. J. Edgcombe, and U. Valdrè, “Some comments on models for field enhancement,”
*Ultramicroscopy*, vol. 95, 57 pages, 2003. View at Publisher · View at Google Scholar - V. Semet, R. Mouton, and V. T. Binh, “Scanning anode field emission microscopy analysis for studies of planar cathodes,”
*Journal of Vacuum Science & Technology B*, vol. 23, no. 2, 671 pages, 2005. View at Publisher · View at Google Scholar - V. Semet, C. Adessi, and V. T. Binh, “Field emission from low barrier surface cathodes,” in
*Proceedings of the 19th International Vacuum Nanoelectronics Conference, and the 50th International Field Emission Symposium (IVNC/IFES '06)*, p. 25, Guilin, China, July 2006. View at Publisher · View at Google Scholar